Download presentation

1
Crystal Structure Lecture 4

2
**The Space Lattice and Unit Cells**

Atoms, arranged in repetitive 3-Dimensional pattern, in long range order (LRO) give rise to crystal structure. Properties of solids depends upon crystal structure and bonding force. An imaginary network of lines, with atoms at intersection of lines, representing the arrangement of atoms is called space lattice. Space Lattice Unit cell is that block of atoms which repeats itself to form space lattice. Materials arranged in short range order are called amorphous materials Unit Cell 3-2

3
**Crystal Systems and Bravais Lattice**

Only seven different types of unit cells are necessary to create all point lattices. According to Bravais ( ) fourteen standard unit cells can describe all possible lattice networks. The four basic types of unit cells are Simple Body Centered Face Centered Base Centered 3-3

4
**Types of Unit Cells Cubic Unit Cell Tetragonal α = β = γ = 900**

a = b = c α = β = γ = 900 Tetragonal a =b ≠ c Body Centered Simple Figure 3.2 Face centered Simple Body Centered 3-4 After W.G. Moffatt, G.W. Pearsall, & J. Wulff, “The Structure and Properties of Materials,” vol. I: “Structure,” Wiley, 1964, p.47.)

5
**Types of Unit Cells (Cont..)**

Orthorhombic a ≠ b ≠ c α = β = γ = 900 Rhombohedral a =b = c α = β = γ ≠ 900 Simple Base Centered Body Centered Face Centered Figure 3.2 Simple 3-5 After W.G. Moffatt, G.W. Pearsall, & J. Wulff, “The Structure and Properties of Materials,” vol. I: “Structure,” Wiley, 1964, p.47.)

6
**Types of Unit Cells (Cont..)**

Hexagonal a ≠ b ≠ c α = β = γ = 900 Monoclinic Triclinic Simple Base Centered Simple Figure 3.2 Simple 3-6 After W.G. Moffatt, G.W. Pearsall, & J. Wulff, “The Structure and Properties of Materials,” vol. I: “Structure,” Wiley, 1964, p.47.)

7
**Principal Metallic Crystal Structures**

90% of the metals have either Body Centered Cubic (BCC), Face Centered Cubic (FCC) or Hexagonal Close Packed (HCP) crystal structure. HCP is denser version of simple hexagonal crystal structure. FCC Structure HCP Structure BCC Structure Figure 3.3 3-7

8
**Body Centered Cubic (BCC) Crystal Structure**

Represented as one atom at each corner of cube and one at the center of cube. Each atom has 8 nearest neighbors. Therefore, coordination number is 8. Examples :- Chromium (a=0.289 nm) Iron (a=0.287 nm) Sodium (a=0.429 nm) Figure 3.4 a&b 3-8

9
**BCC Crystal Structure (Cont..)**

Each unit cell has eight 1/8 atom at corners and 1 full atom at the center. Therefore each unit cell has Atoms contact each other at cube diagonal (8x1/8 ) + 1 = 2 atoms Figure 3.5 Therefore, lattice constant a = 3-9

10
**Atomic Packing Factor of BCC Structure**

Volume of atoms in unit cell Atomic Packing Factor = Volume of unit cell Vatoms = = 8.373R3 V unit cell = a3 = = R3 8.723 R3 Therefore APF = = 0.68 12.32 R3 3-10

11
**Face Centered Cubic (FCC) Crystal Structure**

FCC structure is represented as one atom each at the corner of cube and at the center of each cube face. Coordination number for FCC structure is 12 Atomic Packing Factor is 0.74 Examples :- Aluminum (a = 0.405) Gold (a = 0.408) Figure 3.6 a&b 3-11

12
**FCC Crystal Structure (Cont..)**

Each unit cell has eight 1/8 atom at corners and six ½ atoms at the center of six faces. Therefore each unit cell has Atoms contact each other across cubic face diagonal (8 x 1/8)+ (6 x ½) = 4 atoms Therefore, lattice constant a = Figure 3.7 3-12

13
**Hexagonal Close-Packed Structure**

The HCP structure is represented as an atom at each of 12 corners of a hexagonal prism, 2 atoms at top and bottom face and 3 atoms in between top and bottom face. Atoms attain higher APF by attaining HCP structure than simple hexagonal structure. The coordination number is 12, APF = 0.74. Figure 3.8 a&b 3-13 After F.M. Miller, “Chemistry: Structure and Dynamics,” McGraw-Hill, 1984, p.296

14
**HCP Crystal Structure (Cont..)**

Each atom has six 1/6 atoms at each of top and bottom layer, two half atoms at top and bottom layer and 3 full atoms at the middle layer. Therefore each HCP unit cell has Examples:- Zinc (a = nm, c/a = 1.85) Cobalt (a = nm, c.a = 1.62) Ideal c/a ratio is (2 x 6 x 1/6) + (2 x ½) + 3 = 6 atoms Figure 3.8 c 3-14 After F.M. Miller, “Chemistry: Structure and Dynamics,” McGraw-Hill, 1984, p.296

15
**Atom Positions in Cubic Unit Cells**

Cartesian coordinate system is use to locate atoms. In a cubic unit cell y axis is the direction to the right. x axis is the direction coming out of the paper. z axis is the direction towards top. Negative directions are to the opposite of positive directions. Atom positions are located using unit distances along the axes. Figure 3.10 b 3-15

16
**Directions in Cubic Unit Cells**

In cubic crystals, Direction Indices are vector components of directions resolved along each axes, resolved to smallest integers. Direction indices are position coordinates of unit cell where the direction vector emerges from cell surface, converted to integers. Figure 3.11 3-16

17
**Procedure to Find Direction Indices**

Produce the direction vector till it emerges from surface of cubic cell z (1,1/2,1) - (0,0,0) = (1,1/2,1) (1,1/2,1) Determine the coordinates of point of emergence and origin y (0,0,0) 2 x (1,1/2,1) = (2,1,2) Subtract coordinates of point of Emergence by that of origin x The direction indices are [212] NO Convert them to smallest possible integer by multiplying by an integer. All are integers? YES Are any of the direction vectors negative? NO YES Represent the indices in a square bracket without comas with a over negative index (Eg: [121]) Represent the indices in a square bracket without comas (Eg: [212] ) 3-17

18
**Direction Indices - Example**

Determine direction indices of the given vector. Origin coordinates are (3/4 , 0 , 1/4). Emergence coordinates are (1/4, 1/2, 1/2). Subtracting origin coordinates from emergence coordinates, (1/4, 1/2, 1/2)-(3/4 , 0 , 1/4) = (-1/2, 1/2, 1/4) Multiply by 4 to convert all fractions to integers 4 x (-1/2, 1/2, 1/4) = (-2, 2, 1) Therefore, the direction indices are [ ] Figure EP3.6 3-18

19
Miller Indices Miller Indices are are used to refer to specific lattice planes of atoms. They are reciprocals of the fractional intercepts (with fractions cleared) that the plane makes with the crystallographic x,y and z axes of three nonparallel edges of the cubic unit cell. z Miller Indices =(111) y x 3-19

20
**Miller Indices - Procedure**

Choose a plane that does not pass through origin Determine the x,y and z intercepts of the plane Find the reciprocals of the intercepts Clear fractions by multiplying by an integer to determine smallest set of whole numbers Fractions? Place a ‘bar’ over the Negative indices Enclose in parenthesis (hkl)where h,k,l are miller indicesof cubic crystal plane forx,y and z axes. Eg: (111) 3-20

21
**Miller Indices - Examples**

Intercepts of the plane at x,y & z axes are 1, ∞ and ∞ Taking reciprocals we get (1,0,0). Miller indices are (100). ******************* Intercepts are 1/3, 2/3 & 1. taking reciprocals we get (3, 3/2, 1). Multiplying by 2 to clear fractions, we get (6,3,2). Miller indices are (632). z (100) y x x Figure 3.14 3-21

22
**Miller Indices - Examples**

Plot the plane (101) Taking reciprocals of the indices we get (1 ∞ 1). The intercepts of the plane are x=1, y= ∞ (parallel to y) and z=1. ****************************** Plot the plane (2 2 1) Taking reciprocals of the indices we get (1/2 1/2 1). The intercepts of the plane are x=1/2, y= 1/2 and z=1. Figure EP3.7 a Figure EP3.7 c 3-22

23
**Miller Indices - Example**

Plot the plane (110) The reciprocals are (1,-1, ∞) The intercepts are x=1, y=-1 and z= ∞ (parallel to z axis) To show this plane a single unit cell, the origin is moved along the positive direction of y axis by 1 unit. (110) z y x 3-23

24
**Miller Indices – Important Relationship**

Direction indices of a direction perpendicular to a crystal plane are same as miller indices of the plane. Example:- Interplanar spacing between parallel closest planes with same miller indices is given by z y (110) [110] x Figure EP3.7b 3-24

25
**Planes and Directions in Hexagonal Unit Cells**

Four indices are used (hkil) called as Miller-Bravais indices. Four axes are used (a1, a2, a3 and c). Reciprocal of the intercepts that a crystal plane makes with the a1, a2, a3 and c axes give the h,k,I and l indices respectively. Figure 3.16 3-25

26
**Hexagonal Unit Cell - Examples**

Basal Planes:- Intercepts a1 = ∞ a2 = ∞ a3 = ∞ c = 1 (hkli) = (0001) Prism Planes :- For plane ABCD, Intercepts a1 = 1 a3 = -1 c = ∞ (hkli) = (1010) Figure 3.12 a&b 3-26

27
**Directions in HCP Unit Cells**

Indicated by 4 indices [uvtw]. u,v,t and w are lattice vectors in a1, a2, a3 and c directions respectively. Example:- For a1, a2, a3 directions, the direction indices are [ ], [ ] and [ ] respectively. Figure 3.18 d&e 3-27

28
**Comparison of FCC and HCP crystals**

Both FCC and HCP are close packed and have APF 0.74. FCC crystal is close packed in (111) plane while HCP is close packed in (0001) plane. Figure 3.19 a&b 3-28 After W.G. Moffatt, G.W. Pearsall, & J. Wulff, “The Structure and Properties of Materials,” vol. I: “Structure,” Wiley, 1964, p.51.)

29
**Structural Difference between HCP and FCC**

Plane A Consider a layer of atoms (Plane ‘A’) ‘a’ void ‘b’ void Another layer (plane ‘B’) of atoms is placed in ‘a’ Void of plane ‘A’ Plane A Plane B ‘a’ void ‘b’ void Third layer of Atoms placed in ‘b’ Voids of plane ‘B’. (Identical to plane ‘A’.) HCP crystal. Third layer of Atoms placed in ‘a’ voids of plane ‘B’. Resulting In 3rd Plane C FCC crystal. Plane A Plane A Plane B Plane B Plane A Plane C Figure 3.20 3-29

30
**Volume Density Mass/Unit cell Volume density of metal =**

Example:- Copper (FCC) has atomic mass of g/mol and atomic radius of nm. = Volume/Unit cell a= = = nm Volume of unit cell = V= a3 = (0.361nm)3 = 4.7 x m3 FCC unit cell has 4 atoms. Mass of unit cell = m = = 4.22 x Mg 3-30

31
**Planar Atomic Density Planar atomic density=**

Equivalent number of atoms whose centers are intersected by selected area Planar atomic density= Example:- In Iron (BCC, a=0.287), The (100) plane intersects center of 5 atoms (Four ¼ and 1 full atom). Equivalent number of atoms = (4 x ¼ ) + 1 = 2 atoms Area of 110 plane = = Selected area = Figure 3.22 a&b 3-31

32
**Linear Atomic Density Linear atomic density = =**

Number of atomic diameters intersected by selected length of line in direction of interest Linear atomic density = Example:- For a FCC copper crystal (a=0.361), the [110] direction intersects 2 half diameters and 1 full diameter. Therefore, it intersects ½ + ½ + 1 = 2 atomic diameters. Length of line = = Selected length of line Figure 3.23 3-32

33
**Polymorphism or Allotropy**

Metals exist in more than one crystalline form. This is caller polymorphism or allotropy. Temperature and pressure leads to change in crystalline forms. Example:- Iron exists in both BCC and FCC form depending on the temperature. Liquid Iron -2730C 9120C 13940C 15390C α Iron BCC γ Iron FCC δ Iron BCC 3-33

34
**Crystal Structure Analysis**

Information about crystal structure are obtained using X-Rays. The X-rays used are about the same wavelength ( nm) as distance between crystal lattice planes. 35 KV (Eg: Molybdenum) Figure 3.25 3-34 After B.D. Cullity, “Elements of X-Ray Diffraction, “ 2d ed., Addison-Wesley, 1978, p.23.

35
**X-Ray Spectrum of Molybdenum**

X-Ray spectrum of Molybdenum is obtained when Molybdenum is used as target metal. Kα and Kβ are characteristic of an element. For Molybdenum Kα occurs at wave length of about 0.07nm. Electrons of n=1 shell of target metal are knocked out by bombarding electrons. Electrons of higher level drop down by releasing energy to replace lost electrons Figure 3.26 3-35

36
X-Ray Diffraction Crystal planes of target metal act as mirrors reflecting X-ray beam. If rays leaving a set of planes are out of phase (as in case of arbitrary angle of incidence) no reinforced beam is produced. If rays leaving are in phase, reinforced beams are Figure 3.28 3-36 After A.G. Guy and J.J. Hren, “Elements of Physical Metallurgy,” 3d ed., Addison-Wesley, 1974, p.201.)

37
**X-Ray Diffraction (Cont..)**

For rays reflected from different planes to be in phase, the extra distance traveled by a ray should be a integral multiple of wave length λ . nλ = MP + PN (n = 1,2…) n is order of diffraction If dhkl is interplanar distance, Then MP = PN = dhkl.Sinθ Therefore, λ = 2 dhkl.Sinθ Figure 3.28 3-37 After A.G. Guy and J.J. Hren, “Elements of Physical Metallurgy,” 3d ed., Addison-Wesley, 1974, p.201.)

38
**Interpreting Diffraction Data**

We know that Since Substituting for d, Therefore Note that the wavelength λ and lattice constant a are the same For both incoming and outgoing radiation. 3-38

39
**Interpreting Diffraction Data (Cont..)**

For planes ‘A’ and ‘B’ we get two equations (For plane ‘A’) (For plane ‘B’) Dividing each other, we get 3-39

40
**X-Ray Diffraction Analysis**

Powdered specimen is used for X-ray diffraction analysis as the random orientation facilitates different angle of incidence. Radiation counter detects angle and intensity of diffracted beam. Figure 3.30 3-40 After A.G. Guy “Essentials of Materials Science,” McGraw-Hill, 1976.

41
**Diffraction Condition for Cubic Cells**

For BCC structure, diffraction occurs only on planes whose miller indices when added together total to an even number. I.e. (h+k+l) = even Reflections present (h+k+l) = odd Reflections absent For FCC structure, diffraction occurs only on planes whose miller indices are either all even or all odd. I.e. (h,k,l) all even Reflections present (h,k,l) all odd Reflections present (h,k,l) not all even or all odd Reflections absent. 3-41

42
**Interpreting Experimental Data**

For BCC crystals, the first two sets of diffracting planes are {110} and {200} planes. Therefore For FCC crystals the first two sets of diffracting planes are {111} and {200} planes 3-42

43
**Crystal Structure of Unknown Metal**

Crystallographic Analysis FCC Crystal Structure BCC Crystal Structure 3-43

44
**Random spatial positions of atoms**

Amorphous Materials Random spatial positions of atoms Polymers: Secondary bonds do not allow formation of parallel and tightly packed chains during solidification. Polymers can be semicrystalline. Glass is a ceramic made up of SiO4 4- tetrahedron subunits – limited mobility. Rapid cooling of metals (10 8 K/s) can give rise to amorphous structure (metallic glass). Metallic glass has superior metallic properties.

Similar presentations

OK

STRUCTURE OF SOLID MATERIALS CLASSIFICATION OF SOLIDS SOLIDS CLASSIFIED AS CRYSTALLINE, AMORPHOUS OR A COMBINATION OF THE TWO. CRYSTALLINE - BUILT UP OF.

STRUCTURE OF SOLID MATERIALS CLASSIFICATION OF SOLIDS SOLIDS CLASSIFIED AS CRYSTALLINE, AMORPHOUS OR A COMBINATION OF THE TWO. CRYSTALLINE - BUILT UP OF.

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on corporate social responsibility under companies act 2013 Ppt on food adulteration in india Free download ppt on flow of control in c++ Ppt on direct and indirect speech in english grammar Ppt on how email works Ppt on recent mergers and acquisitions in india Ppt on road accident Ppt on nature and human ads Ppt on brand management Ppt on standing order 2-99